Sulfur has a strong surface activity both in binary (Fe-S) and ternary (Fe-C-S, Fe-Si-S) alloys. It has been concluded from the results of numerous studies that sulfur can exist in two forms in molten iron: in one case it forms an interstitial solutions, and in other partially substitutional solutions. It has been found that the activity of sulfur increase substantially when carbon and silicon are present in the melt. This explains why pig iron can be desulfurized more readily than steel.

Sulfur (S) is a typical metalloid. The radius of sulfur atom is 1.05 Å. It easily acquires two electrons to form an ion S^{2-}. The coefficient of diffusion of sulfur in liquid iron is 0.74x10^{-4}, 13x10^{-4}, 1.9x10_{-5} cm/s, according to various experimental data. Sulfur has a strong surface activity both in binary (Fe-S) and ternary (Fe-C-S, Fe-Si-S) alloys. It has been concluded from the results of numerous studies that sulfur can exist in two forms in molten iron: in one case it forms an interstitial solution, and in other partially substitutional solutions. It has been found that the activity of sulfur increase substantially when carbon and silicon are present in the melt. This explains why pig iron can be desulfurized more readily than steel.

A good understanding of the desulphurization of hot metal and liquid steel has been developed in terms of slag-metal reactions, based on a number of studies of the partition of sulfur between liquid slag and liquid iron. These results show that a highly basic slag, high temperature and reducing conditions enhance desulphurization via slag-metal reactions.

The desulphurization of liquid iron with slag may be examined on the basis of the following reaction (1), in which the equilibrium constant can be expressed by equation (2).

[S] + (O2-) = (S2-) + [O] .......... (1)

log K_{1} = a_{s}^{2-}. a_{o} / a_{s}. a_{o}^{2-} .......... (2)

where,

- a
_{o}, a_{s}: the activities of oxygen and sulfur in liquid iron, respectively - a
_{o}^{2-}, a_{s}^{2-}: the activities of oxygen and sulfur ions in slag, respectively.

The sulfur partition ratio between metal and slag is given by equation (3) according to reaction (1).

L_{S} = (wt%S) / [wt%S] = K_{1} • a_{o}^{2-} • f_{s} / a_{o} • f_{s}^{2-} .......... (3)

where,

- f
_{s}, f_{s}^{2-}: the activity coefficients of sulfur in liquid iron and slag, respectively.

Since the values of K_{1}, a_{o}^{2-} and f_{s}^{2-} cannot be determined experimentally, the sulfide capacity is defined as equation (5) on the basis of reaction (4) and is utilized for the examination of desulphurization in iron and steel making processes.

½ S_{2} + (O_{2-}) = (S^{2-}) + ½ O_{2} .......... (4)

C_{S} = (wt%S) • (P_{O2} / Ps)½ = K_{4} a_{o}2- / f_{s}^{2-} .......... (5)

where,

- P
_{O2}and P_{s}are the oxygen and sulfur partial pressure in atm; - K
_{4}the equilibrium constant of reaction (4).

In order to calculate the value of C_{S}, the equilibrium constants of reactions (6) and (7) are substituted into equation (5), and equation (8) is obtained.

½ O_{2} = [O] .......... (6)

½ S_{2} = [S] .......... (7)

log C_{s} = log (wt % S) a_{o} / a_{s} + 936 / T-1.375 .......... (8)

By the use of the interaction coefficients of sulfur and oxygen in liquid iron, the values of C_{S} can be calculated from equation (8).

As an illustration, the calculation of sulfide capacity (C_{S}) has been given for CaO-MgO-Al_{2}O_{3}-SiO_{2} ladle slags.

In order to examine the relationship between C_{S} and composition of slag, the following relationship is assumed to hold at certain temperatures.

log C_{S} = α (N_{CaO} + K_{MgO} • N_{MgO} + K_{Al2O3}• N_{Al2O3} + K_{SiO2} • N_{SiO2})+ β .......... (9)

where:

- α, β: the constants
- Ni, Ki: the mole fraction and the lime equivalent coefficient of i-component in the slag phase, respectively.

At 1600°C, the values of K_{MgO}, K_{Al2O3} and K_{SiO2} determined by trial and error are 0.1, -0.8 and -1.0, respectively. As shown in Figure 1, there are linear relations between log C_{s} and (N_{CaO} + 0.1 N_{MgO} – 0.8 N_{Al2O3} – N_{SiO2}) at 1575, 1600 and 1650°C.

Figure 1: Plot of the log C_{s} against N_{CaO} + 0.1N_{MgO} – 0.8N_{Al2O3} – N_{SiO2} at 1575, 1600 and 1650°C

The three lines obtained by the method of least squares are shown in the figure. The intercepts of the lines were determined by the use of the slope at 1600°C because the most runs were done at this temperature. The following equation was obtained as a function of temperature.

log C_{S} = 3.44 (N_{CaO} +0.1N_{MgO} – 0.8N_{Al2O3} – N_{SiO2}) - 9894 / T+2.05 .......... (10)

The observed values of log C_{S} with the correlation coefficient (R) of 0.99 and the standard deviation (σ) of 0.044 can well be expressed by the above equation.

On the other hand, log L_{S} may be expressed by the following general equation derived from equations. (3), (8) and (10).

log L_{S} = α ∑ K_{i}•N_{i} - log [wt%O] - β .......... (11)

where,

- ∑ K
_{i}•N_{i}= N_{CaO}+0.1N_{MgO}– 0.8N_{Al2O3}– N_{SiO2}.

The experimental data were arranged by the method of least squares according to equation (11) and the following relationship was obtained.

log L_{S} = 3.44 ∑ K_{i}•N_{i} - log [wt% O] - 10 980 / T+3.50 .......... (12)

Duffy and Ingram defined the theoretical optical basicity (Λ) as follows:

Λ = ∑ (x_{i} / f_{i}) .......... (13)

where, x_{i}, f_{i} : the equivalent cationic fraction and the basicity moderating parameter for the constituent cation i, respectively.

It was verified by them that f_{i} can be expressed by the Pauling's electronegativity x_{i} as follows:

f_{i} =1.36 (x_{i} -0.26) .......... (14)

It was also found by Duffy and Ingram that log C_{S} are linearly correlated to the theoretical optical basicity.

As an illustration of the above mentioned the experimental results performed on ladle CaO-MgO-Al_{2}O_{3}-SiO_{2} slags has been given. The values of log C_{S} are plotted against the optical basicities at 1575, 1600 and 1650°C, as shown in Figure 2.

Figure 2: Plot of log CS against theoretical optical basicity Λ

The slopes and intercepts of the lines were determined by the method of least squares, and the following linear relationship was obtained as a function of temperature.

log C_{S} = 14.20Λ - 9 894 / T -7.55 .......... (15)

As described above, it can be seen that both the sum of lime equivalent and the optical basicity are able to be used as parameters for the representation of sulfide capacity. From the relationship between these two parameters, the linear equation (16) from regression was obtained.

Λ = 0.24(N_{CaO} + 0.1N_{MgO} – 0.8N_{Al2O3} – N_{SiO2}) + 0.67 .......... (16)

The correlation coefficient (R) is larger than 0.99, and the standard deviation (σ) is smaller than 0.01. This shows that the two parameters have almost the same character for the representation of sulfide capacity of slag.

It is well known that the oxygen potential exerts a large influence on the sulfur partition between metal and slag. The equilibrium of reaction (17) was determined by the use of the value of the equilibrium constant (18) reported in literature.

(FeO) = [Fe] + [O] .......... (17)

log K_{17} = log a_{o} / a_{FeO} = -6 150 / T + 2.604 .......... (18)

Equation (18) may be modified to the following equation.

log [wt%O] = log N_{FeO} + log γ_{FeO} - log f_{o} - 6 150 / T + 2.604 .......... (19)

where γ_{FeO} is the activity coefficient of FeO on the basis of mole fraction.

Since log γ_{FeO} is a function of temperature and slag composition, log [wt%O] can be expressed by an equation including the term of log N_{FeO}, then the following relationship was obtained.

log [wt%O] = 0.905 log N_{FeO} -0.15 ∑ K_{i}•N_{i} - 6 340 / T + 3.115 .......... (20)

where, ∑ K_{i}•N_{i} = N_{CaO} + 0.1N_{MgO} – 0.8N_{Al2O3} – N_{SiO2}.

As shown in Figure 3, the observed values of log [wt% O] agree well with the values calculated from the equation (20). By substituting equation (20) into equation (12), equation (21) is derived:

log LS = 3.59 ∑ K_{i}•N_{i} -0.905 log N_{FeO} – 4 640 / T + 0.385 .......... (21)

The above equation can conveniently be used for the estimation of the sulfur partition between liquid iron and slag in which the oxygen content in liquid iron is not analyzed. Next, the values of γ_{FeO} calculated from the equation (19) were arranged by the way similar to that described previously, and the following relationship was obtained.

Figure 3: Comparison of the observed log [wt%O] with calculated log [wt%O] from the equation (20)

Total Materia is the leading materials information platform, providing the most extensive information on metallic and non-metallic material properties and other material records.

All this information is available in Total Materia Horizon, the ultimate materials information and selection tool, providing unparalleled access to over 540,000 materials as well as, curated and updated reference data.

Total Materia Horizon includes:

- Comprehensive data on mechanical, physical properties
- >80 Global standards and their equivalencies
- Precision tools for comparison and analytics streamlining the selection process.
- Stress-strain, formability, fatigue, creep and fracture data
- Exports to over 25 CAx formats.
- Heat treatment, metallography, corrosion information
- Welding, brazing and adhesives data
- Monthly updated, traceable sources ensure reliability

May, 2008

Contact Us

Solve Your Materials Challenges

Find out how we can help